Journal of Cultural Heritage 40 (2019) 163–168
Available online at
MA-XRF imaging as a tool to characterize the 16th century heraldic stained-glass panels in Ghent Saint Bavo Cathedral夽 Stijn Legrand a , Geert Van der Snickt a,b , Simone Cagno a,∗ , Joost Caen b , Koen Janssens a a b
AXES Group, Department of Chemistry, University of Antwerp, Groenenborgerlaan 171, 2020 Antwerp, Belgium Conservation Studies, Heritage Department, Faculty of Design Sciences, University of Antwerp, Blindestraat 9-13, 2000 Antwerp, Belgium
a r t i c l e
i n f o
Article history: Received 31 January 2019 Accepted 11 June 2019 Available online 26 June 2019 Keywords: Glass conservation Macro-imaging MA-XRF Stained-glass windows Chemical imaging
a b s t r a c t MA-XRF is a novel macroscopic imaging technique originally developed for easel paintings and recently made available to glass conservators. This paper discusses the ﬁrst real-life contribution of MA-XRF imaging to a conservation intervention of stained-glass panels. The six panels under study belong to the cathedral building since their creation in 1555–1559 AD. MA-XRF appeared an outstanding tool for ﬁrst-line screening of stained-glass windows, providing readily interpretable information on glass type, coloring and alteration processes. In particular, the chemical imaging technique allowed distinguishing unambiguously the surviving original glass panes from later additions, thereby ensuring a correct historical understanding. From a more practical point of view, the experiments supplied accurate schemes that can be directly incorporated in condition reports and assist designing the ensuing conservation approach. © 2019 Elsevier Masson SAS. All rights reserved.
1. Introduction Correct conservation practice of stained-glass windows includes a complete technical examination of all components, such as the substrate glass of the panels, the glass paints and the lead cames. This is a labor-intensive process and is typically done by visual and microscopic inspection. In a few cases, usually when deterioration or historical issues have to be addressed, this is complemented with chemico-physical analyses. A typical approach involves either sampling or non-invasive point measurement on each pane, for instance with portable XRF, Raman Spectroscopy or PIXE (see e.g. [1–4]). While sampling is disputable in the context of a conservation campaign, in situ analysis is often time and capital intensive, requires interpretation by experienced staff and is always at risk of non-representativity. Time-effective approaches documenting complete windows, in a chemical and organized way, would be particularly welcome, as this would allow assessing the age estimates by connoisseurs, color technology and ongoing alteration processes. Therefore, a few imaging methods have been tested, starting with IR reﬂectography and IR photography, which have been used for preliminary assessment of the state of conservation. However, their scope is limited to surface features and provide no speciﬁcity for glass compositions
. UV–vis–NIR mapping, instead, has been proposed for the investigation of (mainly) colored glasses, but also for the discrimination of different glass compositions . However, in literature only point measurement analyses are reported for stained glass windows . Redox mapping has also been tested for stained glasses, with additional beneﬁt for glass alteration studies, however, this being based at large scale research infrastructures, it is far from applicable in common conservation practice . Macro X-ray Fluorescence (MA-XRF) scanning on the other hand, allows recording compositional data in a completely noninvasive and non-destructive way from the entire object under examination. This data can be presented in distribution images, which are interpretable by a larger public than the spectra resulting from classical spectrometric techniques. A mobile MA-XRF 2D scanning instrument for ﬂat objects has been made available in 2011  and has performed well on (iconic) paintings (see e.g. ). The suitability of MA-XRF as a screening technique for stained-glass windows has recently been proven . While 2D scans are deemed sufﬁcient for most conservation purposes, depth selective data collection by confocal XRF on stained glass windows has also been reported in literature .
2. Research aims 夽 Paper selected from the YOCOCU conference 2018, Matera May 23–25. ∗ Corresponding author. E-mail address: [email protected]
(S. Cagno). https://doi.org/10.1016/j.culher.2019.06.003 1296-2074/© 2019 Elsevier Masson SAS. All rights reserved.
This paper describes the ﬁrst application of macro X-ray ﬂuorescence (MA-XRF) on stained-glass windows in the framework of a real-life conservation-restoration intervention. The six glass
S. Legrand et al. / Journal of Cultural Heritage 40 (2019) 163–168
Fig. 1. The MA-XRF scanning setup in front of the Ryne panel. Glass panels were scanned on their exterior side, while positioned on an easel.
panels object of this study belong to the Saint Bavo Cathedral in Ghent, Belgium. They were selected for MA-XRF scanning measurements since they were assessed by curators to belong to the Saint Bavo Cathedral building as of 1559, and therefore the only known remains of the once impressive historical glazing program of the cathedral. The aim of the study was to provide objective evidence to the conservators on the amount of original glass panes and later additions. The extensive documentation generated with this study, consisting in chemical element distribution maps of the entire panels, is aimed at improving the understanding of the materials and processes used for their manufacture and past restorations. This, in turn, will enable a better preservation of their state of conservation. 3. Materials and methods The six heraldic panels (57 × 60 cm2 ) can be dated between 1555 and 1559 and were part of a window in the St. Landoald side chapel of Ghent Saint Bavo Cathedral. A 17th century manuscript kept in the Rijksarchief Gent shows the entire window and inscriptions, making clear that the window depicted the ‘Resurrection’ surrounded with coats of arms and the representation of the donors. All six surviving panels show typical 16th century heraldic representations: a shield of arms surrounded by decorative scrolls and the name of the family in capital letters (Figs. 1, 2A, 3A). At present, the panels are not in situ, but presented in the sacristy. Visual inspection of the panels suggested that a number of glass panes were probably replaced in the course of past restoration interventions. For these windows, micro-sampling (e.g. under the lead cames) for quantitative SEM-EDX analyses was not permitted, due to the historical relevance of the stained-glass windows. Therefore, all stained-glass panels were analyzed in reﬂection mode by means of the MA-XRF scanning instrument built within the AXES group of the University of Antwerp, more details on the setup can be found elsewhere . The scanner consists of an XRF measurement head mounted on a software-controlled X-Y motor stage with a travel range of about 60 × 57 cm (h × v). The measurement head is equipped with one Vortex EX-90 SDD detector that is positioned in a 20◦ angle with respect to the incident X-ray beam. The X-ray source is a XOS 50 W Rh anode tube. MA-XRF scans were performed by sweeping the
measuring head systematically over the glass surface, respecting a stable distance of ca. 1 cm in between the edge of the measuring head and the panel. The diameter of the primary beam was reduced to a focal spot of 50 m at 4 mm in front of the instrument by implementing a polycapillary X-ray lens. By ofsetting the distance between the optics and the panel, the divergent X-ray beam had an effective spotsize of 700 m. For each pixel in the scanned area, an XRF spectrum is collected. From these spectra, after a spectral ﬁtting process , XRF maps are created for each element detected. The resulting maps, shown in Figs. 2–3, are sometimes gamma/contrast adjusted for better reading. Standard measurement parameters resulted in a total scan time of about 24 hours for each panel. Additional details on measurement conditions are available in . For a more efﬁcient narration, only the ensuing X-ray ﬂuorescence maps, and not the spectra, are shown in the following section. The MA-XRF setup is transportable and can be used at the location where the objects are stored or restored. Performing in situ scans on panels in their architectural setting is feasible as well, but requires supporting structures that allow for safe positioning of the equipment and the absence of physical obstructions that can hamper the movement of the measuring head. In this case, the panels were positioned on an easel for the entire duration of the measurements, while the measuring head moved across the entire surface, as shown by Fig. 1. 4. Results and discussion The results are presented in this section according to the type of information sought. In order to keep the discussion compact, only selected results of the Kethulle and Crane panels are discussed hereafter (see Figs. 2 and 3, respectively). The data was collected from the exterior side, but for the comfort of the reader the ﬁgures are shown reversed. 4.1. Assessment of the state of conservation MA-XRF scans can be used to document (the lack of) structural integrity of the window with a level of detail comparable with the scan resolution. For instance, the X-ray continuum map (Fig. 2M), which is in essence a distribution plot of primary X-rays scattered by the object under study, indicates the presence of chemical elements with low atomic number. In practice, this is especially valid for organic materials such as the polymers or glues (epoxy resins in this case) applied in the framework of a previous conservation treatment. In the current case, the lead-came network and joints are intact, having been replaced in the course of the recent conservation intervention. However, the XRF maps of Pb and Sn in Figs. 2K–L illustrate the potential of the technique to document discontinuities in the lead came network and soldering joints. In this way, MA-XRF can be employed for performing quality checks on the results of a conservation treatment as well. 4.2. Glass composition With these experiments we predominantly aimed at visualizing relative differences in glass composition, allowing distinguishing between modern (i.e., replaced in later instances) and ancient glasses, and between different glassmaking technologies. The grey values of the panes in the maps shown in Figs. 2–3 are relative indications of the concentration of a chemical element. While black panes in the maps imply that element was not detected there, the brighter the tone, the higher is the detected X-ray intensity of that element. Pixel intensities can also be shown as bi-plots (see e.g. the Ca/K bi-plots in Fig. 2D, 3D).
S. Legrand et al. / Journal of Cultural Heritage 40 (2019) 163–168
Fig. 2. A–O: A. Kethulle panel - exterior side; B. K-K XRF map; C. Ca-K XRF map; D. Bi-plot of the K and Ca pixel intensities (a.u.); E. As-K XRF map; F. Mn-K XRF map; G. Ag-L XRF map; H. Fe-K XRF map; I. Co-K XRF map; J. Cr-K XRF map; K. Pb-L XRF map showing the lead came network; L. Sn-L XRF map showing the soldering; M. Continuum map showing in white likely organic material, such as polymeric ﬁller. N. False-color map in function of As/Ca pixel intensity bi-plot. O. False-color map in function of Mn/Ca pixel intensity bi-plot.
Fig. 3. A–K: A. Crane panel - exterior side; B. K-K XRF map; C. Ca-K XRF map; D. Bi-plot of the K and Ca pixel intensities (a.u.); E. As-K XRF map; F. Mn-K XRF map; G. Ag-L XRF map; H. Rb-K XRF map; I. Sr-K XRF map; J. False-color map in function of As/Ca pixel intensity bi-plot; K. False-color map in function of Mn/Ca pixel intensity bi-plot.
S. Legrand et al. / Journal of Cultural Heritage 40 (2019) 163–168
Fig. 4. Window glass compositions commonly used in the Low Countries from 12th century onwards, and their hierarchical classiﬁcation according to their major element content (adapted from ). Lead glass was introduced in England in the late 17th century, sparsely occurring in window glass of the Low Countries. Industrial soda glass appeared in the course of the 19th century, after the invention of synthetic soda, and can be found in case of replacement of glass panes. Vegetable soda and mixed alkali glass rarely occur in window glass, while they are well represented in post-medieval luxury vessel glass. High-lime low-alkali glass and potash glass are the two most widely used compositions for window glass, the ﬁrst with its use peaking between the 12th and the 17th century, and the second between the 12th and the 15th century .
The possible glass families expected to occur in the Saint Bavo Cathedral windows are those used for window glass in the Low Countries in the period 1555-present, i.e. potash glass, high-lime low-alkali (HLLA) glass, lead glass, vegetable ash soda glass and synthetic soda glass, the latter in case of replacements in modern times . These glass families, and their hierarchical classiﬁcation are summarized in Fig. 4. Further information on categories of historical window glass in other contexts can be found, e.g., in [1,15]. As shown in Fig. 4, the chemical elements allowing identifying the glass groups are Na, K, Ca and Pb. However, since MA-XRF experiments are performed in ambient air, the low energy ﬂuorescence radiation emitted by Na is absorbed by air. Therefore, only the K, Ca and Pb distribution maps can be employed to identify these glass groups. No Pb is detected in compatible manner with its presence in the glass matrix, therefore the occurrence of lead glass can be ruled out. When looking at the K distribution maps shown in Figs. 2B and 3B, it is striking how a number of corner panes appear to contain very low/not-detectable levels of potassium. Even if Na is not detectable, a vegetable source of soda (i.e. ash) would carry along an amount of potassium (see Fig. 4). This is a strong indication that the ﬂux used for these panes was high purity synthetic soda, industrially produced from the late 18th century onwards, and used for glass at a large scale from the 19th century. Therefore, such glass panes must have been replaced at a later date. The same panes demonstrate lower intensities of Ca (Figs. 2C, 3C) and higher As levels (Figs. 2E, 3E). Arsenic was used in high quality clear glass from the 18th century onwards, and typically up until the 19th century . The co-existence of synthetic soda glass and arsenic in the replaced panes thus indicates a 19th century intervention. In all the investigated windows between two and four glass panes appear to be made of modern glass.
All original glass appears to contain potassium as main ﬂuxing agent, accompanied by relevant amounts of Ca. This would locate them in the last two categories on the right of Fig. 4 (HLLA glass and potash glass). The assessed composition of the original glass does not contradict the 1555–1559 AD date, as per conservator’s judgment. Being K and Ca adjacent elements, their characteristic X-rays undergo similar attenuation phenomena. By comparing the K/Ca intensities in Figs. 2D–3D, one could attempt a further discrimination between potash and HLLA glass, based on historical glass compositions. The K/Ca intensity ratio appears to be 0.4 or lower, which is comparable with the average K/Ca (0.36) ratio of the most common type of HLLA-glass in use in the Low Countries in the 16th century, and far from the average ratio (0.94) of the most common potash-glass composition . However, these indications would need to be corroborated by analyses on samples. In a second step, pixel intensity bi-plots can be used to identify clusters revealing various correlations between two chemical elements. By assigning user-chosen colors to identiﬁed clusters, false colored grouping of glass panes can be visualized. As an example, in the Kethulle panel (Fig. 2N), two clusters of pixels are found: the ﬁrst (in green) features medium to high levels of calcium and low levels of arsenic, while the second cluster (in red) has lower levels of Ca, positively correlated with As. These clusters correspond to the aforementioned original and replaced glass panes. In the Mn/Ca bi-plot, instead (Fig. 2O), next to a cluster with low Ca and Mn (red), a large group with high Ca and Mn pixels is found (green). These correspond to replaced and original glass, respectively. In addition, a subset of the latter, with intermediate levels of Ca and Mn, can be further distinguished (light blue). These pixels belong to three small panes, with a glass composition compatible with the 16th century, but different from the green group. This could represent an indication of the use of glass of two qualities in the original windows. Two groups of HLLA glass, differentiated by their Mn content (above and below 0.2% MnO) have been
S. Legrand et al. / Journal of Cultural Heritage 40 (2019) 163–168
identiﬁed, for instance, in English windows glass of the 16–17th century . For the Crane panel, similar results are obtained, but in this case, it is clear that a higher amount of original glass panes have been maintained (Fig. 3J–K). 4.3. Glass appearance MA-XRF allowed to identify a single glass-pane (the centre-top pane of the Kethulle window), which is colored by iron, with a lightgreen tint. Since the majority of the panels is made of clear glass, no other pane shows such a uniform distribution of a coloring element (e.g. Mn for purple, or Co for blue glass). While a comparison of MA-XRF data collected from the interior and the exterior side of the windows could also allow differentiation of ﬂashed glass from pot metal glass , in this case the scans were performed from the exterior side only. The introduction of Mn in ancient glass, when not intentional to produce purple color, was meant to counteract the light yellowgreen color caused by Fe impurities in the raw materials [17,18]. In these panels, Mn contents appears variable and allows a further distinction in two groups of original glass, as mentioned in the previous section. The modern panes with low K and high As levels, stand out as well in the Mn maps in Figs. 2F and 3F. This modern clear glass, made with high purity raw materials, did not need manganese addition in its production process. In the outer (original) panes of all windows, the painted decorative border and related decorations are visible at many locations in the Ag XRF maps (Figs. 2G, 3G) and, in negative in the K XRF map (Figs. 2, 3B). This is an indication that silver staining was applied on the exterior side of the window, causing a diffusion of Ag into the glass, and a corresponding depletion of alkali, in this case, potassium . In the Kethulle panel, the star-shaped decoration in the centrebottom pane is visible in negative in the Co (Fig. 2I) and in the Fe map (Fig. 2H), and in positive in Ag map (Fig. 2G). Because of their uneven distribution, it can be deduced that cobalt and iron were applied as glass paints on the exterior side, while the star is obtained by means of silver staining on the exterior side. Moreover, Cr signals were detected in the same glass pane (Fig. 2J), a ﬁnding that is indicative of cold-applied inpainting with modern pigments such as chrome greens, reds and/or yellows. The similar pattern of the Cr to the Co and Fe distributions seems to indicate that all elements were contained in the glass paint used to obtain the resulting brown appearance. Therefore, the investigation of glass colorants can also shed light on previous conservation interventions. 4.4. Glass deterioration During glass weathering the most mobile cations (Na, K) are leached out of the glass surface due to repeated cycles of hydration/dehydration, resulting in the formation of layers of hydrated silica. In parallel, deposits of metal carbonates and sulfates are formed on the glass surface following interaction of these cations with air and atmospheric particulate matter [20–22]. These processes can be observed in the MA-XRF maps as well, through the increased level of calcium that corresponds with the observed pit corrosion craters. Glass alteration might complicate the aforementioned glass type interpretation based on K and Ca ratios. In particular, the weathering can cause a depletion of K or formation of Ca-rich crusts, altering in this way the ratio. However, in case of signiﬁcant weathering, Rb and Sr XRF signals can be used as an alternative for Ca and K [1,2,11]. Rb and Sr are largely co-occurring with K and Ca,
respectively, in the raw materials used to make glass. Being more energetic, their X-ray emission can be detected even when originating from deeper in the glass, i.e. at a depth less likely to be affected by superimposed alteration. As an example, for the Crane panel, Figs. 3B–C can be compared with Fig. 3H–I. 5. Conclusion and outlook In this real-life conservation scenario, MA-XRF supplied relevant chemical information from the entire glass surface in a timeefﬁcient manner. The information provided by the technique is immediately usable by the conservator to answer precise historical and structural questions. In particular, MA-XRF is highly suitable for: • assessing the structural integrity of the window; • distinguishing groups of glass panes with a similar composition and outliers within the same panel; • differentiate glass paints, especially modern ones; • documenting glass alteration. Historical stained-glass panels and windows nearly always contain several later replacement panes and inﬁllings. Quite often it is difﬁcult to date these only by visual examination. MA-XRF revealed unambiguously that about a quarter of the glass panes were replaced, by modern (19th C.) synthetic soda glass containing arsenic. The surviving original glass is likely high-lime low-alkali glass, which is compatible with the presumed dating (1555–1559 AD). The coloring process probably involved a mix of ﬂashed glass, grisaille and glass paint. Modern glass paint was detected, while clear indications of silver staining were found on the original panes. In this way, MA-XRF proved to be an important additional ‘tool’ for the correct dating of stained-glass and as a reliable source of information for conservators and curators. However, the qualitative nature of the technique allows only distinguishing types of panes within the same panel. Exact, quantitative information on the glass composition still requires analysis on samples. Still, it is expected that an increased availability of this technique will favor improved knowledge on the history of stained-glass windows and their state of conservation, and therefore more accurate interventions. Acknowledgements This research was supported by the InBev-Baillet Latour fund. We gratefully acknowledge the Bishop of Ghent and the authorities of Ghent Sint-Baafs Cathedral, who gave the permission to perform this research. References  D. Dungworth, Historic window glass. The use of chemical analysis to date manufacture, J. Archit. Conserv. 18 (2012) 7–25.  L.W. Adlington, I.C. Freestone, Using handheld pXRF to study medieval stained glass: A methodology using trace elements, MRS Adv. 2 (2017) 1785–1800.  M. Walczak, M. Kaminska, P. Karaszkiewicz, J. Szczerbinski, M. Szymonski, The preliminary results on the investigation of historic stained glass panels from Grodziec collection, Poland, Proc. SPIE 8790 (2013), 87901 F-1.  G. Weber, Y. Van den Bemden, M. Pirotte, B. Gilbert, Study of stained glass window using PIXE–PIGE, Nucl. Instrum. Met. Phys. Res. Sect. B 240 (2005) 512–519.  O. Hahn, S. Bretz, C. Hagnau, H.J. Ranz, T. Wolff, Pigments, dyes, and black enamel—the colorants of reverse paintings on glass, Archaeol. Anthropol. Sci. 1 (2009) 263–271.  W. Meulebroeck, P. Cosyns, K. Baert, H. Wouters, S. Cagno, K. Janssens, Optical spectroscopy as a rapid and low-cost tool for the ﬁrst-line analysis of glass artefacts: a step-by-step plan for Roman green glass, J. Archaeol. Sci. 38 (2011) 2387–2398.  W. Meulebroeck, H. Wouters, K. Nys, H. Thienpont, Authenticity screening of stained glasses, Sci. Rep. 6 (2016) [Article number: 37726].
S. Legrand et al. / Journal of Cultural Heritage 40 (2019) 163–168
 M. Hunault, C. Loisel, F. Bauchau, Q. Lemasson, C. Pacheco, L. Pichon, B. Moignard, K. Boulanger, M. Hérold, G. Calas, I. Pallot-Frossardt, Nondestructive redox quantiﬁcation reveals glassmaking of rare French gothic stained glasses, Anal. Chem. 89 (2017) 6277–6284.  M. Alfeld, K. Janssens, J. Dik, W. De Nolf, G. Van der Snickt, Optimization of mobile scanning macro-XRF systems for the in situ investigation of historical paintings, J. Anal. At. Spectrom. 26 (2011) 899–909.  M. Alfeld, J. Vaz Pedroso, M. Van Eikema Hommes, G. Van der Snickt, G. Tauber, J. Blaas, M. Haschke, K. Erler, J. Dik, K. Janssens, A mobile instrument for in-situ scanning macro-XRF investigation of historical paintings’, J. Anal. At. Spectrom. 28 (2013) 760–767.  G. Van der Snickt, S. Legrand, J. Caen, F. Vanmeert, M. Alfeld, K. Janssens, Chemical imaging of stained-glass windows by means of macro X-ray ﬂuorescence (MA-XRF) scanning, Microchem. J. 124 (2016) 615–622.  I. Mantouvalou, K. Aziz-Lange, T. Wolff, D. Grötzsch, L. Lühl, M. Haschke, O. Hahn, B. Kanngießer, A compact 3D Micro X-Ray ﬂuorescence spectrometer with X-ray tube excitation for archaeometric applications, J. Anal. Atom. Spectrom. 25 (2010) 554–561.  G. Van der Snickt, S. Legrand, I. Slama, E. Van Zuien, G. Gruber, K. Van der Stighelen, L. Klaassen, E. Oberthaler, K. Janssens, In situ macro X-ray ﬂuorescence (MA-XRF) scanning as a non-invasive tool to probe for subsurface modiﬁcations in paintings by PP Rubens, Microchem. J. 138 (2018) 238–245.  M. Alfeld, K. Janssens, Strategies for processing mega-pixel X-ray ﬂuorescence hyperspectral data: a case study on a version of Caravaggio’s painting Supper at Emmaus, J. Anal. Atom. Spectrom. 30 (30) (2015) 777–789.
 O. Schalm, K. Janssens, H. Wouters, D. Caluwé, Composition of 12-18th century window glass in Belgium: Non-ﬁgurative windows in secular buildings and stained-glass windows in religious buildings, Spectrochim. Acta B 62 (2007) 663–668. ˙  J. Kunicki-Goldﬁnger, L. Kierzek, P. Dzierzanowski, A.J. Kasrzak, “Central European crystal glass of the ﬁrst half of the eighteenth century.” In: Annales du 16e Congrès de l’Association Internationale pour l’Histoire du Verre, Nottingham: AIHV, 2005, pp. 258–262.  A. Ceglia, G. Nuyts, W. Meulebroeck, S. Cagno, A. Silvestri, A. Zoleo, K. Nys, K. Janssens, H. Thienpont, H. Terryn, Iron speciation in soda lime silica glass: a comparison of XANES and UV–vis–NIR spectroscopy, J. Anal. Atom. Spectrom. 30 (2015) 1552–1561.  R. Arletti, S. Quartieri, I.C. Freestone, A XANES study of chromophores in archaeological glass, Appl. Phys. A Mater. Sci. Proc. 111 (2013) 99–108.  D. Jembrih-Simbuerger, C. Neelmeijer, O. Schalm, P. Friedricks, M. Schreiner, K. De Vis, M. Maeder, D. Schryvers, J. Caen, The colour of silver stained glass–analytical investigation carried out with XRF, SEM/EDX, TEM and IBA, J. Anal. Atom. Spectrom. 17 (2002) 321–328.  G. Nuyts, S. Cagno, S. Bugani, K. Janssens, Micro-XANES study on Mn browning: use of quantitative valence state maps, J. Anal. Atom. Spectrom. 30 (2015) 642–650.  M. Schreiner, Glass of the past: The degradation and deterioration of medieval glass artifacts, Microchim. Acta 104 (1991) 255–264.  H. Roemich, S. Gerlach, P. Mottner, F. Mees, P. Jacobs, D. Van Dyck, T. Carbo, Scientiﬁc Basis for Nuclear Waste Management XXVI, 2003, pp. 97–108 (506 Keystone Drive, Warrendale, PA 15088-7563 USA).